How to cite this paper: Menezes-Silva, R., Reis, L.A., Tostes, B.O., Douglas de Oliveira, D.W. and Santos, M.H. (2015) Bond Strength of Brackets Bonded with Chemically and Light Activated Materials after Thermal Cycling. AdvancesinMaterials PhysicsandChemistry, 5, 351-360. http://dx.doi.org/10.4236/ampc.2015.59035
Bond Strength of Brackets Bonded with
Chemically and Light Activated Materials
after Thermal Cycling
, Leonardo Amaral dos Reis2
, Bhenya Otonni Tostes1
Dhelfeson Willyan Douglas de Oliveira3
, Maria Helena Santos4
1Department of Dentistry, Endodontics and Dental Materials, Bauru Dental School, University of São
Paulo—USP, Bauru, Brazil
2Department of Pathology, Piracicaba Dental School, University of Campinas—UNICAMP, Piracicaba, Brazil 3Department of Dentistry, Federal University of Minas Gerais—UFMG, Belo Horizonte, Brazil
4Department of Dentistry, Federal University of the “Vales do Jequitinhonha e Mucuri”—UFVJM, Diamantina,
Received 28 July 2015; accepted 30 August 2015; published 2 September 2015
Copyright © 2015 by authors and Scientific Research Publishing Inc.
This work is licensed under the Creative Commons Attribution International License (CC BY).
The aim of this study was to evaluate the bond strength of orthodontic brackets bonded to tooth enamel with different polymer composites after simulated clinical aging, and analyze the enamel/ bond system fracture interface. 80 human premolars, were randomly divided into five groups (n = 16). G1: CO (Concise Ortodôntica—3M ESPE), G2: SB (SuperBond—Ortho Source), G3: FMO (Fill Magic Ortodôntico—Vigodent), G4: TXT (Transbond XT—3M ESPE) and G5: TP (Transbond Plus Self Etching Primer + Transbond Plus Color Change—3M ESPE). In all groups, the metal orthodon-tic bracket was bonded to the tooth enamel surface. The specimens were submitted to 3000 ther-mal cycling baths for 30 s, at temperatures of 5˚C, 37˚C and 55˚C (±1˚C). Afterwards they were sub-jected to shear testing and the results were analyzed by the Student’s-t test (p < 0.05). G1 pre-sented the highest bond strength value, followed by G4 > G5 > G2 > G3. In all groups the majority of the fractures at the interface of the specimens were cohesive, except in G3, which presented the largest number of adhesive fractures. After clinical aging, the chemically activated material (CO) showed higher bond strength than the light activated types (FMO, TXT and TP). The self-etching adhesive system (TP) showed similar bond strength to that of conventional systems (FMO and TXT).
Dental Bonding, Orthodontic Brackets, Orthodontics
In the oral cavity, orthodontic brackets are subject to innumerable forces. These may be concentrated in the ad-hesive layer, or at the adad-hesive/enamel interface, compromising bracket retention  . The bond strength of brackets is influenced by the physical and mechanical properties of the polymer cementing materials, adverse conditions of humidity and temperature present in the mouth, design of the mesh of the bracket base, and me-thod of enamel etching -. In the present study, cementing materials and adhesive systems were evaluated in order to find the best option of material and technique, which would guarantee functional results satisfactory to the patient, without harming the integrity of the tooth.
The progressive technological development of polymer materials associated with acid etching and adhesive systems have provided a wide variety of options of polymer composites on the dental market over the years. For orthodontic bracket bonding there are both chemically and light-activated resins available on the market. Nev-ertheless, a study evaluating the bond strength of resin composites pointed out a better performance of the che- mically activated, in comparison with the light activated types .
With so many options on the market, the orthodontist may find it difficult to select and acquire the material that really provides the best properties, and that would be the correct indication for a clinical step in orthodontic correction as important as bracket bonding.
In view of the foregoing, the aim of this study was to evaluate the bond strength of metal orthodontic brackets bonded to tooth enamel with chemically and light-activated materials, and submitted to clinical aging. For this purpose, after cementation and thermal cycling, shear bond strength tests were performed; the structural and elemental characteristics of the surface of materials and enamel/adhesive system/bracket interfaces, as well as the depth of adhesive system penetration into the enamel were analyzed.
The present experiment received approval from the Animal Experimentation Ethics Committee of the Federal University of the Jequitinhonha and Mucuri (Brazil) under registration number 050/09.
A total of eighty first premolars recently extracted due to orthodontic indication were collected, cleaned and stored in distilled water at 6˚C. The selected teeth were examined in order to guarantee that they were free of cracks or other defects in the enamel that could possibly affect the results.
The teeth were randomly divided into five groups (n = 16). Each tooth was involved with polyester resin up to the cement-enamel junction. The study groups were identified according to the bracket cementing material. The names, composition and manufacturers of the products used are shown in Chart 1.
After prophylaxis of the vestibular surfaces of the teeth, a metal edgewise bracket, reference 10.30.208 (Mo-relli, Sorocaba, SP, Brazil), was bonded to the tooth enamel by a same trained operator (RMS), in accordance with the recommendations of each cementing material manufacturer.
In G3, G4 and G5 groups the resin materials were light activated using the LED light appliance (Ultralux EL, Dabi Atlante, Ribeirão Preto, SP, Brazil), at the power from 350 to 500 mw/cm2. In G1 and G2 groups, the resin materials were chemically activated.
Previously to resin cementation, markings were made in the central region of the vestibular surface, by visual method, in order to standardize the position of the brackets in the occlusal-gingival and mesio-distal directions.
All the specimens were stored in distilled water at 37˚C. After 30 days, they were submitted to 3000 thermal cycling baths in a thermal cycling machine (MSCT/3e–ELQUIP, São Paulo, SP, Brazil).Alternately, 30 s-baths were performed for each temperature (5˚C ± 1˚C, 37˚C ± 1˚C and 55˚C ± 1˚C), with an interval of 5s between each bath.
Chart 1. Chart of identification of groups, characteristics of the materials used for acid etching enamel and cementing brackets, with their commercial brands and respective manufacturers.
Group n = 16 Trademark Conditioning enamel Material cementing
G1 Concise Ortodôntica (CO)
(3 M ESPE)
Phosphoric acid 37% (Scotchbond—3 M ESPE)
Chemically actived cementing agent
G2 SuperBond (SB)
Phosphoric acid 35% (Superbond—Ortho Source)
Chemically actived cementing agent
G3 Fill Magic Ortodôntico
Phosphoric acid 37% (Magic acid—Vigodent)
Light actived cementing agent
G4 Transbond XT (TXT) Phosphoric acid 37%
(Unitek—3 M ESPE)
Light actived cementing agent
Transbond Plus Self Etching Primer
+ Trasbond Plus Color Change (TP)
(3 M) (ESPE)
Self-etching cementing agent +
Light actived cementing agent
The interfaces of the specimens were examined under a stereoscopic microscope Stemi 2000C (Carl Zeiss), at 16× magnification, to determine the type of fracture. The fractures were classified as follows : adhesive— fracture at the resin/adhesive interface; cohesive in enamel—fracture in the tooth enamel structure; cohesive in resin—fracture in the resin cylinder body; mixed—fracture involving resin and/or adhesive and/or tooth structure.
Test specimens representative of each group were randomly selected and sectioned along their long axis, in the vestibular-lingual direction. The mesial and distal sections were immersed in hydrochloric acid (HCL) (6 mol/l) for 30 s . Dehydration was performed, using increasing concentrations of acetone. The dehydrated sections were sputter-coated with a thin layer of gold-palladium, and analyzed by a scanning electron micro-scope (SEM) (CS-3500, Shimadzu, Japan) and a Energy dispersive X-ray spectroscopy (EDS) (CS3200, Oxford, England).
Data analysis was performed with the Statistical Package for Social Sciences (SPSS version 22.0, IBM Inc., USA). Descriptive statistics were performed. The Shapiro-Wilk test and Levene’s test were used for the deter-mination of normality and equality of variance, respectively. The results of bracket bond strength were submit-ted to the One-Way ANOVA with Student's t test as posthoc test. The level of significance was set at 95% (p< 0.05).
The bond strength values of this study are showed in Table 1.
The predominant type of fracture in G1, G2, G4 and G5 groups was cohesive in resin. The G3 group pre-sented the highest number of adhesive fractures. No damage to the enamel surface was observed after debonding, with the exception of two samples from G1, which presented fracture in enamel (Graphic 1).
The SEM photomicrographs images suggested that the largest particles were observed in CO (Figures 1(A)), followed by G2 (Figures 1(B)). The resins FMO (Figure 1(C)), TXT (Figure 1(D)) and TP (Figure 1(E)) were shown to be more homogeneous in the particle size of its filler. From the images it was possible to observe a fa-vorable distribution of inorganic particles in the organic matrix, without the occurrence of agglomerations in the large majority of materials.
CO/enamel interface showed a thick and uniform hybrid layer along the entire extension of the bracket bond-ing area with the formation of small tags in the enamel (Figure 1(a)). The SB resin showed a thinner hybrid layer and smaller tags (Figure 1(B) andFigure 1(b)). The hybrid layer formed with the use of FMO (Figure 1(C)) and TXT (Figure 1(D)) shown to be thinner. At higher magnification, the transition zone between the ad-hesive layer and demineralized enamel of FMO and TXT may be observed inFigure 1(c) andFigure 1(d), re-spectively. The TP resin showed a thinner hybrid layer and smaller tags, and more continuous, thicker and uni-form (Figure 1(E) and Figure 1(e)).
Figure 1. SEM photomicrographs of resin/enamel interfaces at 200× and 1000× magnifications: G1-CO ((A) and (a)), G2-SB ((B) and (b)) and G3-FMO ((C) and (c)), G4-TXT ((D) and (d)) and G5-TP ((E) and (e)).
Graph 1. Graph representative of fracture types at enamel/cementing agent interface after the shear bond strength test.
Table 1.Representative table of the values of bond strength to the enamel of the materials used for bonding brackets.
Bond strength (MPa)
Group Mean SD p* Post-hoc**
G1 22.25 10.71 A
G2 14.85 5.17 AB
G3 11.63 7.7 0.010 B
G4 15.12 8.3 AB
G5 14.92 7.68 AB
ANOVA. **test t-student (p < 0.05).
with high intensity peaks of Si, in addition to carbon (C) and oxygen (O). The characteristic peaks of these ma-terials may be observed in the spectrum of G1 (Figure 2(a)). Its spectra in areas of the hybrid layer also showed the same pattern and may be represented by spectrum of G3 (Figure 2(b)). The hybrid layer spectra of G2 (Figure 2(c)) and G5 (Figure 2(d)) presented Si inside the prism of etched enamel.
An orthodontic resin must be capable of retaining the brackets firmly bonded to the teeth throughout treatment, resisting masticatory forces and those generated by orthodontic mechanics  . However, it is important for orthodontists to know the properties and technique used with materials, in order to prevent bond eventual failures that may lead to bracket debonding, causing loss of efficiency in tooth movement, in addition to time and economic loss to the orthodontist. The present results show that all resin presented bond strength to enamel above the acceptable values for the use in cases of orthodontic bracket bonding. Also, the current results rein-force the idea of the individuality of clinical cases.
The effects of aging caused by thermal cycling have negative consequences on bond strength repair, in com-parison with non-thermal cycled samples, irrespective of the composite and enamel conditioning applied  . Davidson etal. , examined the durability of the shear bond strength of some adhesive systems after they had been submitted up to 300 thermal cycles and observed a significant reduction in bond strength. Price etal., 
Figure 2. EDS Spectra of G1 - CO (a), showing peaks of Si, C and O, representing the EDS spectra of all the groups; hybrid layer area of G3-FMO (b) presenting peaks of Ca, Si and Al, C and O; hybrid layer of G2-SB (c) presenting peaks of Ca, Si, C and O; hybrid layer of G5-TP (d)
showing peaks of Si.
As well as Evans and Powers , also maintained control on bonding to avoid excesses, pressing the brack-ets against the tooth surface. According to these authors’ report, there is a gradual reduction in the bond strength of resins, as the thickness of composites under the devices is increased. Comparing the results of this study with the reference values, it was found that all the adhesive materials presented adequate bond strength for clinical use. The higher values of bond strength to the enamel of the used materials may be attributed to the etching ac-tion of phosphoricacid, which offers the advantage of increased bond strength. However, phosphoric acid etch-ing is able to cause a greater degree of enamel loss .
After the shear bond strength tests, the predominant type of fracture in CO, SB, TXT and TP was cohesive in resin, corroborating the studies of Penido etal.  and Buyukyilmaz etal. . However, in invivo studies, these authors verified that the bond failure occurred at the cement/bracket interface, and that this type of fracture is frequently found in clinical practice. It is the most desirable type, since facture at this interface may cause damage to the enamel, due to strangulation of the resin that remains between the bracket mesh, making this area more fragile . Two samples from CO presented enamel fracture, a result similar to that found by Penido etal.
. Only FMO presented mostly adhesive fractures. Also, there were mixed fractures in all groups that might be the result of mechanical retention of the bracket base or chemical bonding between the enamel and adhesive. Bond failure at any of the mentioned interfaces has its own advantages and disadvantages. For instance, bond failure at the bracket-adhesive interface is advantageous because it leaves an intact enamel surface; however removing residual adhesive is time consuming and imposes the risk of enamel damage. On the other hand, bond failure at the enamel-adhesive interface leaves less residual adhesive remnants but the risk of enamel surface damage is increased. Bond failure at the enamel-adhesive interface leaves less adhesive remnants on the enamel surface and therefore decreases the risk of enamel damage during adhesive removal but imposes a higher risk of enamel damage during debonding . Because of the higher bond strength of CO composite, the risk of enamel damage during debonding is high as well.
Microstructural analysis by SEM showed the differences between the shape, size and disposition of inorganic particles in all the resin materials. CO and SB had larger particles distributed in the organic matrix, and FMO, TXT and TP had smaller and more homogeneous particles. In addition, penetration of all the resin cementing agents into enamel was observed, with tag and hybrid layer formation, the latter being thicker in SB, followed by TXT and FMO. The hybrid layer was thinner in SB; probably, the high viscosity of the product may have made it difficult for the resin to penetrate into the pores. The hybrid layer obtained in TP was more continuous, thicker and uniform.
However, tags are considered fundamental for retention of the material, and responsible for sealing the sur-face, with consequent reduction in marginal leakage . For bracket bonding with the use of different bonding agents, tag and hybrid layer formation are not directly related to its retention to the enamel surface  . In CO, the etched enamel and use of this composite, together with a liquid resin probably allowed more favorable conditions for resin penetration, resulting in a better bond.
The TP Self Etching Primer system is more conservative when compared with the conventional system with phosphoric acid. Because it is self-etching, this adhesive system has high demineralizing capacity and favors adequate bond strength for orthodontic bracket bonding, presenting similar strength to that obtained with phos-phoric acid etching  . A uniform and continuous hybrid layer was observed when associated with the TP Color Change adhesive system. In addition to satisfactory bond strength to enamel and minimization of marginal leakage, simplification of the bonding procedure, significant reduction in clinical time, and bracket removal without harm to the enamel surface, appear to be factors making it advantageous to use this association.
All the groups presented mean values of bond strength to enamel above the acceptable values for the use of or-thodontic bracket bonding. The study allows one to affirm that the resins SB, FMO, TXT and TP attained excel-lent bond strength values. Chemically activated resin composite CO presented higher value of bond strength to enamel than the light activated resin materials FMO, TXT and TP. As regards adhesive systems, there appears to be no difference, because the self-etching system TP demonstrated bond strength similar to that of the conven-tional bonding systems FMO and TXT.
 Correr Sobrinho, L., Correr, G.M., Consani, S., Sinhoreti, M.A.C. and Consani, R.L.X. (2002) Influence of Post-Fixa- tion Time on Shear Bond Strength of Brackets Fixed with Different Bonding Materials. PesquisaOdontológica
Brasi-leira, 16, 43-49.
 Pithon, M.M., Dos Santos, R.L., de Oliveira, M.V., Ruellas, A.C. and Romano, F.L. (2006) Metallic Brackets Bonded with Resin-Reinforced Glass Ionomer Cements under Different Enamel Conditions. AngleOrthodontist, 4, 700-704.  Bengtson, N.G., Bengtson, A.L., Carvalho, D.S. and Rossetto, S.M.A. (2003) Comparative Study of Brackets Bond
 Danielle, M.P., Fábio, L.R., Ary, S.P., Lídia, P.M. and Darcy, F.N. (2005) Analysis of the Adhesion Quality of Differ-ent Metallic Bracket. RevistaDentalPressdeOrtodontiaeOrtopediaFacial, 10, 88-93.
 Melo, T.R.N.B., Maia, A.M.A., Cavalcanti, A.L., Nascimento, A.B.L. and Valença, A.M.G. (2006) Avaliação da resistência ao cisalhamento de adesivos monocomponentes em dentes bovinos. Odontologia Clínico-Científica, 5, 275-280.
 Mondelli, A.L. and Feitas, M.R. (2007) Comparative Study of the Shear Bond Strength of the Resin/Bracket Interface, Using Three Different Resin Composites and Three Different Treatments in the Base of the Bracket. RevistaDental
PressdeOrtodontiaeOrtopediaFacial, 12, 111-125. http://dx.doi.org/10.1590/S1415-54192007000300012
 Isber, H., Ambrosio, A.R., Carvalho, P.E.G., Valle-Corotti, K.M. and Siqueira, D.F. (2011) Comparative inVitro
Study of the Shear Bond Strength of Brackets Bonded with Restorative and Orthodontic Resins. BrazilianOral
Re-search, 25, 49-55.
 International Standards Organization. ISO Standard 11405:2003: Dental Materials-Testing of Adhesion to Tooth Structure. The Organization, Geneva, 2003.
 Fowler, C.S., Swartz, M.L., Moore, B.K. and Rhodes, B.F. (1992) Influence of Selected Variables on Adhesion Testing.
DentalMaterials, 8, 265-9. http://dx.doi.org/10.1016/0109-5641(92)90097-V
 Nakabayashi, M. and Takarada, K. (1992) Effect of HEMA on Bonding to Dentin. DentalMaterials, 8, 125-130.
 Bishara, S.E., Vonwald, L., Laffoon, J.F. and Jakobsen, J.R. (2000) Effect of Altering the Type of Enamel Conditioner on the Shear Bond Strength of a Resin-Reinforced Glass Ionomer Adhesive. American Journalof Orthodonticsand
DentofacialOrthopedics, 118, 288-294. http://dx.doi.org/10.1067/mod.2000.104903
 Reynolds, I.R. (1975) A Review of Direct Orthodontic Bonding. BritishJournalofOrthodontics, 2, 171-180.
 Rinastiti, M., Ozcan, M., Siswomihardjo, W. and Busscher, H.J. (2011) Effects of Surface Conditioning on Repair Bond Strengths of Non-Aged and Aged Microhybrid, Nanohybrid, and Nanofilled Composite Resins. ClinicalOral
Investigations, 15, 625-633. http://dx.doi.org/10.1007/s00784-010-0426-6
 Davidson, C.L., Abdalla, A.I. and De Gee, A.J. (1993) An Investigation into the Quality of Dentin Bonding Systems for Accomplishing a Durable Bond. JournalofOralRehabilitation, 20, 291-300.
 Price, R.B., Derand, T., Andreou, P. and Murphy, D. (2003) The Effect of Two Configuration Factors, Time, and Thermalcycling on Resin to Dentin Bond Strengths. Biomaterials, 24, 1013-1021.
 Evans, L.B. and Powers, J.M. (1985) Factor Affecting inVitro Bond Strength of No-Mix Orthodontic Cements.
Amer-icanJournalofOrthodontics, 87, 508-512. http://dx.doi.org/10.1016/0002-9416(85)90087-9
 Kawakami, R.Y., Pinto, A.S., Gonçalves, J.R., Sakima, M.T. and Gandini, L.G. (2003) InVitro Evaluation of De-bonding Pattern in Bonding Interface of Orthodontic Adhesive Materials to Impacted Teeth Enamel: 48-Hour and 10- Day Shear Bond Strengths. RevistaDentalPressdeOrtodontiaeOrtopediaFacial, 8, 43-61.
 Correr Sobrinho, L., Consani, S., Sinhoretti, M.A.C., Correr, G.M. and Consani, R.L.X. (2001) Evaluation of Shear Bond Strengths of Bracket Bonding Using Different Materials. RevistaABONacional, 9, 157-162.
 Beech, D.R. and Jalaly, T. (1981) Clinical and Laboratory Evaluation of Some Orthodontic Direct Bonding Systems.
JournalofDentalResearch, 60, 972-928. http://dx.doi.org/10.1177/00220345810600061201
 Ianni, F.D., Silva, T.B.C., Simplício, A.H.M., Loffredo, L.C.M. and Ribeiro, R.P. (2004) Shear Bond Strength—In Vi-tro—Evaluation of Different Orthodontics Adhesive. RevistaDentalPressdeOrtodontiaeOrtopediaFacial, 9, 9-48.  Newman, G.V., Snyder, W.H. and Wilson Jr., C.E. (1968) Acrylic Adhesives for Bonding Attachments to Tooth
Sur-faces. TheAngleOrthodontist, 38, 12-18.
 Penido, S.M.M.O., etal. (1998) Shear Resistance Evaluation of Recycled Brackets and New Rebonding Brackets.
Re-vistaDentalPressdeOrtodontiaeOrtopediaFacial, 3, 45-51.
 Buyukyilmaz, T., Usumez, S. and Karaman, A.I. (2003) Effect of Self-Etching Primers on Bond Strength: Are They Reliable. TheAngleOrthodontist, 73, 64-70.
 Nkenke, E., Hirschfelder, U., Martus, F. and Eberhard, H. (1997) Evaluation of the Bond Strength of Different Brack-et-Bonding Systems to Bovine Enamel. EuropeanJournalofOrthodontics, 19, 259-270.
 Penido, S.M.M.O., Penido, C.V.S.R., Pinto, A.S., Sakima, T. and Fontana, C.R. (2008) InVivo and inVitro Study, with or without Thermocycling, of Shear Bond Strength of Brackets Bonded with Halogen Light. RevistaDentalPress
deOrtodontiaeOrtopediaFacial, 13, 66-76. http://dx.doi.org/10.1590/S1415-54192008000300009
Com-posite Resin for Orthodontic Bracket Bonding. JournalofDentistry, 11, 282-289.
 Swift Jr., E.J., Perdigão, J. and Heymann, H.O. (1995) Bonding to Enamel and Dentin: A Brief History and State of the Art. QuintessenceInternational, 26, 95-110.
 Fjeld, M. and Ogaard, B. (2006) Scanning Electron Microscopic Evaluation of Enamel Surfaces Exposed to 3 Ortho-dontic Bonding Systems. AmericanJournalofOrthodonticsandDentofacialOrthopedics, 130, 575-581.
 Montasser, M.A., Drummond, J.L., Roth, J.R., Al-Turki, L. and Evans, C.A. (2008) Rebonding of Orthodontic Brack-ets. Part II: An XPS and SEM Study. TheAngleOrthodontist, 78, 537-544. http://dx.doi.org/10.2319/022707-102.1
 Cal-Neto, J.P. and Miguel, J.A. (2006) Scanning Electron Microscopy Evaluation of the Bonding Mechanism of a Self-Etching Primer on Enamel. TheAngleOrthodontist, 76, 132-136.
 Banks, P. and Thiruvenkatachari, B. (2007) Long-Term Clinical Evaluation of Bracket Failure with a Self-Etching Primer: A Randomized Controlled Trial. JournalofOrthodontics, 34, 243-251.